Anisotropic thermal expansion of La(n)(Ti,Fe)(n)O(3n + 2) (n = 5 and 6)
Wölfel, Alexander; Dorscht, Philipp; Lichtenberg, Frank; van Smaalen, Sander; Acta Crystallographica, Section B: Structural Science, Crystal Engineering and Materials 69 (2013) 137–144; doi:10.1107/S2052519213003126

data_2310738
_publ_section_title
;
 Anisotropic thermal expansion of La(n)(Ti,Fe)(n)O(3n + 2) (n = 5 and 6)
;
_journal_coden_ASTM              ACSBDA
_journal_coeditor_code           BP5048
_journal_issue                   2
_journal_name_full
;
 Acta Crystallographica, Section B: Structural Science, Crystal
 Engineering and Materials
;
_journal_page_first              137
_journal_page_last               144
_journal_paper_doi               10.1107/S2052519213003126
_journal_volume                  69
_journal_year                    2013
_chemical_formula_sum            'Fe0.615 La3.333 O11.333 Ti2.718'
_chemical_formula_weight         808.8
_space_group_IT_number           14
_space_group_ssg_name            X21/b(\a\b0)00
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc (-1/4*x+1/2*z,1/2*x,y)'
_symmetry_space_group_name_H-M   'P 1 21/c 1 (2*c,2*a+c,b)'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.007(17)
_cell_formula_units_Z            1
_cell_length_a                   7.8339(17)
_cell_length_b                   5.2222(15)
_cell_length_c                   5.5444(13)
_cell_measurement_temperature    250
_cell_modulation_dimension       1
_cell_volume                     226.82(10)
_diffrn_ambient_temperature      250
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.94
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0449
_diffrn_reflns_av_sigmaI/netI    0.0219
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_index_m_1_max 6
_diffrn_reflns_limit_index_m_1_min -5
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            58927
_diffrn_reflns_theta_full        34.01
_diffrn_reflns_theta_max         36.49
_diffrn_reflns_theta_min         2.6
_exptl_absorpt_coefficient_mu    18.62
_exptl_crystal_density_diffrn    5.919
_exptl_crystal_F_000             178
_refine_diff_density_max         4.63
_refine_diff_density_min         -3.21
_refine_ls_extinction_coef       1370(60)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    2.79
_refine_ls_goodness_of_fit_ref   2.72
_refine_ls_number_constraints    8
_refine_ls_number_parameters     146
_refine_ls_number_reflns         6510
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0357
_refine_ls_R_factor_gt           0.0332
_refine_ls_shift/su_max          0.0061
_refine_ls_shift/su_mean         0.0005
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0479
_refine_ls_wR_factor_ref         0.0481
_reflns_number_gt                6146
_reflns_number_total             6510
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            bp5048sup1.cif
_cod_data_source_block           n5_250K
_cod_database_code               2310738
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 12
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0